hardwood lumber and veneer series - purdue .hardwood lumber and veneer series daniel l. cassens,
Post on 07-Sep-2018
Embed Size (px)
Hardwood Lumber and Veneer Series
Daniel L. Cassens, Professor and Extension Wood Products Specialist Department of Forestry and Natural Resources, Purdue University, West Lafayette, IN 47907
White oak is truly the all American wood. Dense, strong, durable, and from a long-lived tree, it welcomed the settlers to the east coast. It was used for durable bottom logs in cabins, ships, and most importantly for wagons. As a major component of wagon wheels and other high-strength parts, it carried the settlers even further west and supplied both the North and South with the means to transport artillery and other heavy items used in the Civil War. As the country continued to develop, the last of the old growth timber was sawed into quartered and rift white oak. It was used for the Arts and Crafts movement and Mission Style furniture and to decorate railroad passenger cars. Quartered and rift oak was an important point of contention in the creation of the National Hardwood Lumber Association (NHLA). Today, white oak remains a valuable timber species for both decorative and industrial applications. The time honored phrase, solid as the oak is our own USA surely refers to this species.
White Oak is a term used in the lumber trade that refers to a category of lumber that may contain as many as eight different eastern species of trees. Several additional, mostly non-commercial species, are found in the west.
The multiple species that comprise the white oak lumber category grow in various locations through-out the eastern United States (see Table 1). The first species listed in the table is the preferred one and constitutes three quarters of all the white oak lumber produced. It ranges from the great plains east except the gulf coastal plains and the far northeastern
states. Trees with particularly large plates of flaky bark are some-times referred to as forked-leaf white oak. There are other white oak species, only about one-half of which are significant in the lumber trade. Bur oak is common in both bottomlands and in prairie regions. Its wood is usually a darker brown in color and the wood grain sometimes has a scalloped
White oak tree and Dan Cassens
Hardwood Lumber White Oak
appearance. Chinkapin oak can produce good quality lumber, but it is irregular in occurrence. The wood may have a very light greenish tint. Several other species can be developed into saw-log size material, but the yield of high-grade lumber may be less than the more preferred species.Wood Color and Texture
White oak wood color can vary from a very light straw color, which is currently preferred, to a brown color. The wood can also be mottled with gray. Occasionally, slow growth old trees will produce boards with a pink color, very similar to red oak.
White oak lumber has a very characteristic showy, coarse grain pattern just somewhat more subdued than red oak. White oak is ring porous, which means that in the spring of the year it produces very large diameter pores that are visible to the naked eye. At some point during the growing season, it abruptly begins to produce very small diameter, thick-walled pores. The result is alter-nating layers of coarse and fine textured wood. The pores of the heartwood are also filled with tyloses making the wood impermeable. On a freshly cut surface, the tyloses in the pores will glisten as light reflects off their surface.
All of the oaks have very large wood rays. In fact, these rays are the largest of any North American commercial lumber species. When oak is flat sawn, only the ends of the rays are exposed, and they are relatively inconspicuous in comparison to the large pores. When the lumber is quarter sawn, the boards are cut on a radius from the pith, or very center of the tree, to the bark. The saw is cutting parallel to the large wood rays, and a very characteristic splotchy pattern results. The rays may average 1 inches tall. Rift cut oak results when the rays are intersected at a 45o angle. In this situation, the ends of the rays appear somewhat larger than in flat sawn lumber; but more importantly, the wood appears pencil stripped as the alternating large earlywood pores run parallel to the small dense latewood pores. The industry prefers to sell quartered and rift cut oak together. Quartered and rift oak was commonly used in Mission Style furniture and during the Arts and Crafts period. The appearance is strictly different than that of flat-sawn oak.
WorkabilityWhite oak is rated as one of the very best woods
for planing, shaping, turning, and boring. It is a hard wood but tends to cut clean without tearing or fuzzying.Strength
At 12 percent moisture content, white oak will weigh about 47 pounds per cubic foot making it the heaviest lumber species next to hickory. With the exception of bur oak, which is somewhat weaker, it is one of our strongest species.
White oak has excellent mechanical or strength properties. These properties can vary somewhat by species. Considering failure in bending (MOR) and shear strength, the values for true white oak are considerably higher than Douglas fir or loblolly pine. In bending, or MOE, the three species are about equal. However, the wood of white oak is much heavier and harder to nail than that of Douglas fir and southern pine.Steam Bending
In a U.S. Forest Products Laboratory study, white oak is rated one of the very best woods for bending.Drying
White oak lumber is difficult to dry, and a mild kiln schedule must be used. Freshly cut lumber can surface check within a day or less when exposed to the hot summer sun or when air drying proceeds too rapidly. Later in the drying process, internal checks, or honeycomb, can develop if the process proceeds too rapidly. Honeycomb usually occurs in the dry kiln, but it can occur on the air drying yard as well. Commercial producers are aware of these drying problems and follow procedures to avoid them.Shrinkage
As one of our heaviest woods, white oak also has the highest shrinkage next to hickory. However, once properly dried and placed in a stable environment, the wood should have little movement.Decay Resistance
Depending on species, white oaks are rated as resistant or very resistant to moderately resistant to decay. True white oak and bur oak are considered durable, and the wood has had specific applications because of this attribute.
Hardwood Lumber White Oak
Commercial Use, Grading, and ValueWhite oak closely parallels red oak in most
characteristics but has some additional attributes. White oak constitutes about 15 percent of the lumber cut. Together with red oak, these two species groups account for 48 percent of all hardwood lumber produced.
White oak is preferred for interior decorative applications ranging from furniture (especially church furniture), cabinets, millwork, and caskets to hardwood flooring. It is also a very dense strong wood making it a favorite for industrial applications such as railroad ties; mine timbers; pallets; blocking; industrial, agricultural, and truck flooring; and others. As a naturally durable wood, it is also used where this attribute is important. Examples include fence posts, fence boards, sill plates, trailer beds, mine timbers, and railroad ties. Old time uses for white oak include wagon wheels and bottom logs on cabins where rain water splash and subsequent decay create problems.
White oak is the one hardwood species group produced in large quantities of naturally durable lower grade material, which could be used for some construction purposes. There is also a separate price schedule in the Appalachian region where worm
holes are not considered a defect (WHND). The material is low cost and often specified where the strength and durability of oak is needed but a defect free appearance is not required.
Tyloses block the vessels in white oak to any liquid movement making the wood impenetrable to preservatives. Therefore, one unique use of white oak is for tight cooperage such as whiskey barrels and wine casks. Red oak, which normally lacks or has limited tyloses, is not used for tight cooperage, but treats well with liquid preservatives.
White oak lumber when sold as flat-sawn stock is graded standard with the exception that some mineral stain is allowed; but when excessive, it will reduce a board one grade only. When quarter sawn, the minimum board width is reduced from 6 to 5 inches wide.
White oak, in the wholesale market, is usually priced somewhat less than red oak but still considered a valuable species. Veneer quality logs and lumber are commonly exported to Europe as a substitute for European white oak.
Quarter- and rift-sawn white oak is a specialty item and commands a substantial premium compared to standard lumber.
Table 1. Scientific and common names, range, and preferred sites for white oak species growing in the eastern United States
Common and Scientific Names Range Site CommentsWhite oak Quercus alba L.
States bordering the west side of the Mississippi River and then east and S. Canada
Uplands Premier species
Bur oak Q. macrocarpa Mickx.
E. great Plains and E. to Appalachains except southeastern United States, also in S. Canada
Uplands and bottomlands
Acceptable species but wood is dark colored
overcup oak Q. lyrata Walt.
Lower Mississippi and Ohio River bottoms, portions of Atlantic and Gulf coastal states
Bottomlands Poor species
Post oak Q. stellata Wangenh.
Southern portions of eastern and central states and south and then southwest into Texas, Oklahoma, and S.E. Kansas
Dry uplands Poor species
swamp chestnut oak Q. michauxii Nutt.